ACOUSTIC ABSORPTION OF GEOPOLYMER/SAND MIXTURE
IVANA PERNÁ, TOMÁŠ HANZLÍČEK, PAVEL STRAKA, MICHAELA STEINEROVÁ
Institute of Rock Structure and Mechanics of the Academy of Sciences of the Czech Republic, v.v.i.,
V Holesovickach 41, 182 09 Prague, Czech Republic
Submitted June 19 2008; accepted November 5, 2008
Keywords: Acoustic absorption coefficient, Geopolymer
The article describes the acoustic absorption coefficient of material formed by geopolymer joining agent filled by sand. The
geopolymer defined as a clay based inorganic poly-condensed 3D net was used as a substitute of epoxide resin, currently
industrially used cementing material of granular media (generally quartz sand). The absorption coefficient α of conven-
tionally used epoxide/sand sample was compared with studied geopolymer/sand mixtures. The main target was to find the
alternative joining matter caused by permanently bumping costs of epoxide resin and its flammability. Presented paper
deals with the influence of filling agent in geopolymer matrix (quantity of sand and its fractionation) on course of acoustic
absorption coefficient and describes also the influence of thickness of geopolymer/sand mixture. The acoustic absorption
coefficient α was defined within the range from 100 Hz to 2500 Hz. The results showed that both presented mixtures have
specific sound absorbing properties – average value of coefficient with boarder range of effectiveness and high absorbing
coefficient with narrow profile of effective frequencies.
INTRODUCTION space in between sand particles, which finally defined
the acoustic absorption coefficient. Industrially the epoxi-
The noise is defined as undesirable sound, annoying de content does not exceed 8 wt.% and even the formats
and disturbing people in some cases even detrimental. 40 × 40 cm tiles (boards) with thickness of 20 mm
Oversized noise negatively influences human beings only have sufficient flexible resistance allowing the
and their life e.g. health, psyche, hearing and also application on the ceilings.
performance in work. The occurrence of civilization The main target of the presented paper was to
diseases cast by noise was proved by research works find possible alternative joining agent of chosen and
and studies , which also accenting the necessity to industrially used quartz grains and study its coefficient
decrease the unhealthy influence of noise. [α]. Instead of organic polymer–epoxide resin, the study
Common sound decreasing method is, among presents inorganic, geopolymer binding agent joining the
others, the utilization of sound absorbing materials. same grained sand.
The level of sound absorption could be characterized Geopolymers are named by J. Davidovits in 1979
by the absorption coefficient (α) which corresponds to . Geopolymer is based on alkali treated of thermally
the amount of striking energy absorbed on the material activated clay, which forms in ambient conditions 3D
surface. Values α strongly vary with frequency ranging net capable encapsulate in its predominantly amorphous
from 0 to 1, where zero signs that material has no structure the high amount of different materials. The
absorption and α = 1 means full sound absorption. source of geopolymer is generally double layered clay
In the case of bonded granular media, the most im- material, e.g. kaolin. The thermal treatment adjust
portant is managed distribution of homogenously spread alumina ions to desirable position (Al3+ in IV-fold
graded grains in cementing media (e.g. epoxide resins). oxygen coordination) where is possible their hydration
The granular structure has high open interconnected and progressive netting with silica ions. The four oxygen
porosity which causes the transformation of sound waves surrounding around the Al3+ ion result in negative charge
into energy (sound absorption). Lot of articles documents of alumina tetrahedron, which is balanced by alkalis
the acoustic properties of mentioned sound absorbing [13, 14]. The geopolymer is generally insoluble and
materials and their behavior tested by different effects stabile materials with compact microstructure. It has
[2-5]. Many papers present the utilization of mathematical high early strengths, excellent mechanical properties
acoustic modeling [6-8], but only few of them describe comparable with other inorganic binder (Portland ce-
the influence of filler particle sizes and used fractions on ment, gypsum, lime). Appreciable properties are also
acoustic properties [9-12]. fire and heat resistance (up to 1200°C), absence of the
Commonly epoxide bounded sand joins the spherical hazardous combustion gasses and structure stability at
grains among them by cervices, leaving enough free high temperatures [14-18].
48 Ceramics – Silikáty 53 (1) 48-51 (2009)
Acoustic absorption of geopolymer/sand mixture
The investigation of the acoustic absorption coeffi- in Table 2 is only recapitulation of the best results,
cient of geopolymer/sand mixtures show alternative which were accompanied by the set of samples with
binder for industrials. The research results represent firm insufficient industrial requirements. The previous five
and long time collaboration with industrial producer years experiments with different type of geopolymer
of sound absorbing materials and than the specific studies have assured the perfect homogenization when
requirements of application play inconsiderable role. the food processor is used. The homogenized mixture
was after next 10 minutes pulled to the standard cylinder
moulds – diameter 62 mm. After 24 hours, samples were
EXPERIMENTAL removed from moulds and cured at room temperature.
The samples were left at laboratory temperature and
The bounding properties of geopolymers are pressure for 28 days, than tested, defining the acoustic
lower than these of epoxide binder. The amount of absorption coefficient. The Table 2 presents the content
geopolymer has to reach as minimum 20 wt.% of final of geopolymer base, mica and fraction of quartz sand in
tested product; otherwise the flexible resistance is lower wt.%.
than comparable epoxide/sand sample. The presented The parallel sample made from epoxide/sand mix-
paper study the acoustic properties of geopolymer/ ture (8 wt.% of epoxide resin and mono-fraction of
sand mixture but have to reflect on the second plan the sand, diameter 0.3-0.6 mm) was a standard industrial
industrially requirements as flexible resistance, costs and production sample with thickness of 30 mm.
availability of sand fractions. Newly the very important The chemical analyses were performed by an XRF
is also fire resistance. The collaboration with first Czech analyzer (Spectro IQ, Kleve, Germany, where the target
producer - SONING A.S. also orientated the chose of material is palladium, target angle 90° from the central
raw material for geopolymer matrix production to the ray and the focal spot a 1 mm × 1 mm square, the maxi-
secondary sources of clayed materials . mum Anode Dissipation 50 Watts with 10 cfm forced air
According to the previous knowledge and experi- cooling). The sound absorption coefficient was obtained
ments was used NW-Org. clay from the Kamenna Panna by measurement on Brüel & Kjǽr, type 4206 impedance
deposit, Central Bohemia, Czech Republic (highly tube by the transfer-function method according the Inter-
kaoli-nitic refractory clay, containing about 3 wt.% national Standard ISO 10534-2 . The values were
of organic matter and due to this content refused by measured in the range from 100 Hz to 2500 Hz according
ceramic industry). To improve of geopolymer mixture to the most desirable interest of users of sound protecting
properties (lowering the porosity) was added mica dust panels and sheets (measurement level is considered as
to the geopolymer matrix. Used mica dust was from the ± 3.0 % of presented value).
production of insulating mica materials (company Cogebi
A.S., Tábor, Czech Republic). Chemical compositions
RESULTS AND DISCUSSION
are presented at Table 1. The quartz sand was delivered
by Sklopísek Střeleč, a.s. company, Czech Republic, The study presents the results of acoustic absorp-
exploited from sedimentary sandstone deposit. tion coefficient of geopolymer/sand mixture and influen-
The 50 g of activated clay material were mixed ce of its changes due to the thickness and sand fractiona-
by ordinary food kitchen processor with alkaline tion of the samples. The presented Geo 1 mixture is a
activator prepared from NaOH, soluble sodium silicate result of studies which as close as possible copied the
and water. Reaction starts during 25-30 minutes and parallel mixture of epoxide/sand. The official sound
than the mica and after next 5 minutes the sand were laboratory demands for sample testing their thickness of
added. The amount of admixed materials presented 10 and 30 mm.
Table 1. Chemical composition of used material (wt.%).
Material SiO2 Al2O3 Fe2O3 TiO2 CaO MgO K 2O Na2O L.O.I
NW org. 43.59 34.66 1.39 1.44 0.14 < 0.02 0.82 < 0.02 17.33*
Mica 46.02 34.35 2.83 0.42 < 0.002 4.74 10.91 < 0.11 0.1
* the value includes 3 % of organic matter
Table 2. Composition of prepared geopolymer/sand mixtures.
Samples Geopolymer base Mica* Quartz sand with fraction: Quartz sand with fraction:
name (wt.%) (wt.%) 0.3-0.6 mm (wt.%) 0.6-1.2 mm (wt.%)
Geo 1 20 3 77 0
Geo 2 20 3 19 58
* addition of waste mica dust lowered the porosity and is a result of previous experiments
Ceramics – Silikáty 53 (1) 48-51 (2009) 49
Perná I., Hanzlíček T., Straka P., Steinerová M.
The Figure 1 presents the absorption coefficients coefficient of Geo 2 and referenced epoxide/sand mixture
(frequencies from 100 Hz to 2500 Hz) of samples Geo at frequency of 1600 Hz we could reveal only very small
1 in standard thicknesses 10 mm and 30 mm. The curve difference. The peak of epoxide/sand mixture curve is
Geo 1 - thickness 30 mm showed rapid increase in low at frequency 1600 Hz and its coefficient reaches value
values of frequency and from 600 Hz is moderated. The α = 0.83. The acoustic properties of material Geo 2 made
maximum absorption coefficient α is 0.69 (1250 Hz). from two different fractions of sand appear equivalent to
The Geo 1 - thickness 10 mm line showed how the epoxide/sand mixture.
absorption properties could be modified by the change
of thickness only. The increase is slower and the maxi-
mum moves to higher value - 2000 Hz (α = 0.74).
According to the nature of curve, we could suppose
that absorption coefficient could decrease very slowly
and material could be used in sound protection for
frequencies up to 1600 Hz.
The Geo 2 mixture is a result of experimental sets,
where the proportions of bigger and smaller grains
of sand were changed. The best result from the point
of view sound absorption and mechanical property is
presented. The low flexible resistance of the thickness
of 10 mm samples claimed the necessity to prepare
the sample thickness of 20 mm. The following Figure
2 than compares the 20 and 30 mm thickness of Geo 2
Figure 1. Absorption coefficient of geopolymer/sand mixture
mixture. The use of two different fractions of quartz sand Geo 1 (fraction of quartz sand 0.3-0.6 mm).
improves maximum absorption coefficients (α = 0.86-
0.87) but at once sharpens courses of curves and limit
the range of utilization. The maxima are in 1250 Hz and
2000 Hz for thicknesses 30 mm and 20 mm respectively.
Comparing the Geo 2 – thicknesses 30 mm and
20 mm we could find similar behavior as in case of
Geo 1. The thickness of 30 mm composites have maxi-
mum absorption coefficient in same value of frequency
– 1250 Hz.
The industrial requirements mentioned above exclu-
ded all mixtures with:
a) small amount of sand – then the final 77 wt. % is
b) higher quantity of geopolymer matrix then chosen
20 wt. % means lowering the porosity and in the mean
time low sound absorption, Figure 2. Absorption coefficient of geopolymer/sand mixture
c) also lower quantity of geopolymer matrix then men- Geo 2 (fractions of quartz sand 0.3-0.6 mm and 0.6-1.2 mm).
tioned parameter means insufficient flexible resis-
We found also that especially in case of higher
quantities of geopolymer joining agent than mentioned
20 wt. %, that samples or final products are highly
influenced by technique of preparation. The technology
should exclude the vibration of products due to the
thixotropic behavior of geopolymer composition with
high content of sand.
The following Figure 3 shows courses of absorption
coefficient α of the best data of chosen mixtures in range
from 200-2600 Hz – each one (Geo 1 and Geo 2) as a
result of separate series of mixtures and comparison
with industrially prepared standard. The highest value of
absorption coefficient has material Geo 2 with maximum Figure 3. Overview of Geo 1, Geo 2 and epoxide/sand mixture
α = 0.87 at frequency 1250 Hz. Comparing the absorption results of absorption coefficient (thickness of 30 mm).
50 Ceramics – Silikáty 53 (1) 48-51 (2009)
Acoustic absorption of geopolymer/sand mixture
The Figure 3 summarizes the results of absorption The sand bonded by geopolymer resembles very
coefficient of three samples (thickness of 30 mm). The geo- porous natural sandstone but advantages of the tech-
polymer composites Geo1, Geo 2 are compared with stan- nique of geopolymer allow the change and manage
dard 30 mm industrially obtained epoxide/sand mixture. the porosity. Different fractions of quartz sand, their
The curve of Geo 1 shows that mono-fractional sand amount and quantity of geopolymer matrix could easily
material does not reach the values of absorption coeffi- modified acoustic properties according to the various
cient as Geo 2 does, and also the comparable epoxid/sand applications. The application of sound protective tiles
shows better value of α coefficient. The difference could and sheets in the interior of building the newly presents
be the reflex of porosity resulting from mono-fractioned demand of fire resistance. The open flame and fire means
quartz sand. The contact of small grains with minimum fatal consequences (collapse and total destruction) on
of inter-space vacancies results in lower acoustic resis- epoxide/sand products.
tance. Identical amount of joining agent in case of Geo 1 Besides confirming the acoustic property of geopo-
and Geo 2 mixtures differs by fractionation of sand (the lymer/sand mixtures we have acknowledged their fire
influence of 3 wt.% of mica dust on porosity is minimal) resistance up to 1200°C. The industrials which have
in geopolymer surroundings. Important could be a fact to resolve the problem of production costs could apply
that at low frequencies up to approx. 500 Hz the values perspective technology of geopolymers.
α are comparable among all three samples.
The Geo 2 mixture presents better result at frequen-
cies from 1000-1200 Hz but at higher frequencies Acknowledgement
values, over 1600 Hz, the epoxide/sand mixture shows Scientific Research Plan No.AVOZ 30460519 of the
better sound property. The necessary, 3 times higher, Institute of Rock Structure and Mechanics approved by
amount of joining agent (20 wt.%) is "equilibrated" by
Czech Academy of Sciences supported this work.
the combination of two sand fractions. The pores, their
shape and quantity are decisive for the determination
of acoustic property defined by absorption coefficient. References
We could imagine than the space among mentioned 1. Lercher P.: Environ. Int. 22, 117 (1996).
proportion (58 wt.%) of bigger concave grains (from 2. Attenborough K.: J. Acoust. Soc. Am. 73, 785 (1983).
0.6-1.2 mm) is only partially filled by smaller grains 3. Laukaitis A.: Mater. Sci. 4, 58 (1997)
(19 wt.%). The geopolymer joining agent homogenously 4. Horoshenkov K. V., Hughes D. C., Cwirzen A.: Appl.
spread among the grains left sufficient "free" space and Acoust. 64, 197 (2003).
5. Champoux Y., Stinson M. R.: J. Acoust. Soc. Am. 92, 1120
than the porous structure. But experiments also showed (1992)
that required flexible strength orders to double the 6. Voronina N. N., Horoshenkov K. V.: Appl. Acoust. 64, 415
thickness as mentioned above – from 10 to 20 mm. (2003).
The incomparable quality of geopolymer joining 7. Atalla N., Sgard F.: J. Sound Vibr. 303, 195 (2007).
agent is its fire resistance. The purely inorganic basement 8. Voronina N.: Appl. Acoust. 42, 165 (1994).
of alumina–silicates was in presented experiment com- 9. Pfretzschner J., Rodriguez R. M.: Polym. Test 18, 81 (1999).
10. Vašina M., Hughes D.C., Horoshenkov K. V., Lapčík L. Jr:
pleted by use of powdered mica, but the resistance of Appl. Acoust. 67, 787 (2006).
geopolymer itself to high temperatures (up to 1200°C) is 11. Swift M. J., Bris P., Horoshenkov K. V.: Appl. Acoust. 57,
well known. 203 (1999).
12. Park S. B., Lee B. I., Lim Y. S.: Cem. Concr. Res. 21, 589
13. Davidovits J.: J. Therm. Anal. Calorim. 37, 1633 (1991)
14. Xu H., Van Deventer J. S. J.: Int. J. Miner. Process. 59, 247
The results showed that geopolymer/sand mixtures 15. Van Jaarsveld J. G. S., Van Deventer J. S. J., Lukey G. C.:
have good absorption properties and confirm possibility Chem. Eng. J. 89, 63 (2002).
to substitute the industrially used epoxide resin binder 16. Palomo A., Grutzeck M., Blanco M. T.: Cem. Concr. Res.
by geopolymer based matrix. Mono-fractional sand in 29, 1323 (1999).
17. Perna I., Steinerova M., Hanzlicek T., Straka P. in: Advances
combination with geopolymer creates broader range
in Geomaterials and Structure, p.773-777, Ed. Darve F. et
of effectiveness in point of frequencies but absorption al., Hammamet 2006.
coefficient reaches only average value (α = 0.69-0.74). 18. Sanz J., Madani A., Serratoza J. M.: J. Am. Ceram. Soc. 71,
The combination of two different sand particles causes C-418 (1988).
improvement of absorption coefficient up to α = 0.87 19. Hanzlicek T., Perna I., Steinerova M., Straka P. in:
but falls sharply down from 1600 Hz. In case of Geo 2 Proceedings of XXIII. IMPC, 3: p.2273-2276, Ed. Önal
G. et al., Istanbul Technical University, Mining Faculty,
was found that combination of two quartz sand fractions
bounded by 20 wt.% of geopolymer creates adequate 20. International Standard ISO 10534-2:1998. Acoustics-Deter-
open porosity, which finally reveals similar acoustic mination of sound absorption coefficient and impedance in
absorption as referenced epoxide/sand product. impedance tubes-Part 2: Transfer-function method.
Ceramics – Silikáty 53 (1) 48-51 (2009) 51